Standard Specification for Steel, Sheet and Strip, Hot-Rolled, Carbon, Structural, HighStrength Low-Alloy, High-Strength...
]Ù]Ù ][¢ [Ù¢
www.bab ake.n et
Designation: A 1011/A 1011M – 07
Standard Speciﬁcation for
Steel, Sheet and Strip, Hot-Rolled, Carbon, Structural, HighStrength Low-Alloy, High-Strength Low-Alloy with Improved Formability, and Ultra-High Strength 1 This standard is issued under the ﬁxed designation A 1011/A 1011M; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A superscript epsilon (e) indicates an editori editorial al change since the last revision or reapproval.
1. Scope Scope* *
High-Strength Low-Alloy, and High-Strength Low-Alloy with Improved Formability, General Requirements for A 749/A 749M Speciﬁcation for Steel, Strip, Carbon and High-Strength, Low-Alloy, Hot-Rolled, General Requirements for A 941 Terminology Relating to Steel, Stainless Steel, Related Alloys, and Ferroalloys E 18 Test Test Met Method hodss for Roc Rockwe kwell ll Har Hardne dness ss of Met Metall allic ic Materials
1.1 This speciﬁcation covers hot-rolled, hot-rolled, carbon, structural, high-strength high-streng th low-a low-alloy lloy,, highhigh-stren strength gth low-a low-alloy lloy with improved formability, formability, and ultra-high strength steel sheet and strip, in coils and cut lengths. 1.2 Hot rolled rolled ste steel el she sheet et and str strip ip is ava availa ilable ble in the designations as listed in 4.1 4.1.. 1.3 This speciﬁcation is not applicable applicable to the steel covered by Speciﬁcation A Speciﬁcation A 635/A 635M. 635M. 1.4 The values stated in either inch-pound inch-pound units or SI units are to be regarded separately as standard. Within the text, the SI uni units ts are sho shown wn in bra bracke ckets. ts. The val values ues stated stated in eac each h system are not exact equivalents; therefore, each system must be used independently of the other.
3. Terminology 3.1 Deﬁnitions—For deﬁnitions of other terms used in this speciﬁcation refer to Terminology A 941. 941. 3.2 Deﬁnitions of Terms Speciﬁc to This Standard: 3.2.1 aging—loss of ductility with an increase in hardness, yield yiel d stren strength, gth, and tensi tensile le stre strength ngth that occur occurss when steel, which whi ch has been sli slight ghtly ly col cold d wor worked ked (such as by tem temper per rolling) is stored for some time. 18.104.22.168 Discussion—Aging also increases the tendency toward stretcher strains and ﬂuting. 3.2.2 stabilization—a —add ddit itio ion n of on onee or mo more re ni nitr trid idee or carbid car bidee for formin ming g ele elemen ments, ts, or bot both, h, suc such h as tit titani anium um and columbium colu mbium,, to contr control ol the level of the interstitial interstitial elements elements carbon and nitrogen in the steel. 22.214.171.124 Discussion—Stabilization improves formability and increases resistance to aging. 3.2.3 vacuum degassing—process of reﬁning liquid steel in which the liquid is exposed to a vacuum as part of a special technique tech nique for remo removing ving impurities impurities or for deca decarburi rburizing zing the steel.
2. Referenced Documents 2.1 ASTM Standards: 2 A 370 Test Methods and Deﬁnitions for Mechanical Testing of Steel Products A 568/A 568M Spec Speciﬁca iﬁcation tion for Stee Steel, l, Sheet Sheet,, Carbo Carbon, n, Structural, and High-Strength, Low-Alloy, Hot-Rolled and Cold-Rolled, General Requirements for A 569/A 569M Speciﬁcation for Steel, Carbon (0.15 Maximum, Percent), Hot-Rolled Sheet and Strip Commercial 3 A 622/A 622M Speciﬁcation for Drawing Steel (DS), (DS), Sheet 3 and Strip, Carbon, Hot-Rolled A 635/A 635M Speciﬁ Speciﬁcat cation ion for Ste Steel, el, She Sheet et and Str Strip, ip, Heavy-Thickness Coils, Hot-Rolled, Carbon, Structural,
1 This speciﬁcation is under the jurisdiction of ASTM Committee A01 on Steel, Stainless Steel and Related Alloys and is the direct responsibility of Subcommittee A01.19 on Steel Sheet and Strip. Current edition approved Sept. 1, 2007. Published September 2007. Originally approved appr oved in 2000 2000.. Last prev previous ious edition approved approved in 2006 as A 101 1011/ 1/ A 1011M – 06b. 2 For referenced ASTM standards, visit the ASTM website, www.astm.org, or contact ASTM Customer Service at [email protected]
For Annual Book of ASTM volume information, refer to the standard’s Document Summary page on Standards volume Standards the ASTM website. 3 Withdrawn.
4. Classiﬁcation 4.1 Hot-rolled steel sheet and steel strip is available available in the following designations: 4.1.1 Commercial Steel (CS Types Types A, B, C, and D), 4.1.2 Drawing Steel (DS Types Types A and B), NOTE 1—CS 1—CS Type Type B and DS Type B des descri cribe be the most common common product prev product previousl iously y inclu included, ded, resp respectiv ectively ely,, in Spec Speciﬁca iﬁcations tions A A 569/ A 569M and 569M and A A 622/A 622M. 622M.
*A Summary of Changes section appears at the end of this standard. Copyright © ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States.
A 1011/A 1011M – 07 4.1.3 Structural Steel (SS grades 30, 33, 36 Types 1 and 2, 40, 45, 50, 55, 60, 70, and 80), 4.1.4 High-Strength Low-Alloy Steel (HSLAS, classes 1 and 2, in grades 45, 50, 55, 60, 65, and 70. 4.1.5 High-Strength Low-Alloy Steel with Improved Formability (HSLAS-F grades 50, 60, 70, and 80). 126.96.36.199 HSLAS-F steel has improved formability when compared to HSLAS. The steel is fully deoxidized, made to a ﬁne grain practice, and includes microalloying elements such as columbium, vanadium, and zirconium. The steel shall be treated to achieve inclusion control. 4.1.6 Ultra-High Strength (UHSS Types 1 and 2, in Grades 90  and 100 ). 188.8.131.52 UHSS steel has increased strength compared with HSLAS-F. The steel is killed and made to a ﬁne ferritic grain practice, and includes microalloying elements such as columbium (niobium), titanium, vanadium, molybdenum, and so forth. The steel shall be treated to achieve inclusion control. The material is intended for miscellaneous applications where higher strength, savings in weight, and weldability are important. Atmospheric corrosion resistance of these steels is equivalent to plain carbon steels. With copper speciﬁed, the atmospheric corrosion resistance is somewhat enhanced. 4.1.7 When required for HSLAS, HSLAS-F, and UHSS steels, limitations on the use of one or more of the microalloy elements shall be speciﬁed on the order.
NOTE 2—Not all producers are capable of meeting all the limitations of the thickness tolerance tables in Speciﬁcations A 568/A 568M and A 749/ A 749M. The purchaser should contact the producer prior to placing an order.
5.1.7 Coil size (inside diameter, outside diameter, and maximum weight), 5.1.8 Copper bearing steel (if required), 5.1.9 Quantity, 5.1.10 Application (part identiﬁcation and description), 5.1.11 Special requirements (if required), and 5.1.12 A report of heat analysis will be supplied, if requested, for CS and DS. For materials with required mechanical properties, SS, HSLAS, HSLAS-F, and UHSS, a report is required of heat analysis and mechanical properties as determined by the tension test. NOTE 3—A typical ordering description is as follows: ASTM A 1011-XX, hot rolled steel sheet, CS Type A, pickled and oiled, cut edge, 0.075 by 36 by 96 in., thickness tolerance Table 4 of Speciﬁcation A 568/A 568M, 100 000 lb, for part no. 6310, for shelf bracket. or: ASTM A 1011M-XX, hot rolled steel sheet, CS Type B, pickled and oiled, cut edge, 3.7 by 117 mm by coil, ID 600 mm, OD 1500 mm, max weight 10 000 kg, thickness tolerance Table A1.1 of Speciﬁcation A 568/ A 568M, 50 000 kg, for upper control arm.
6. General Requirements for Delivery 6.1 Material furnished under this speciﬁcation shall conform to the applicable requirements of the current edition of Speciﬁcation A 568/A 568M for sheets and Speciﬁcation A 749/A 749M for strip, unless otherwise provided for herein. 7. Chemical Composition
5. Ordering Information
7.1 The heat analysis of the steel shall conform to the chemical composition requirements of the appropriate designation shown in Table 1 for CS and DS and Table 2 for SS, HSLAS, HSLAS-F, and UHSS. 7.2 Each of the elements listed in Tables 1 and 2 shall be included in the report of the heat analysis. When the amount of copper, nickel, chromium, or molybdenum is less than 0.02 %, report the analysis as